# Rectangular nanoplatelets

Dans le document The DART-Europe E-theses Portal (Page 106-112)

## 5.4 Square and rectangular nanoplatelets

### 5.4.2 Rectangular nanoplatelets

5.4.2.1 Polarized emission

Since the emission from some square nanoplatelets is found to be slightly polarized (less than 10%), it can be assumed that such a weak polarization may due to a slightly rectangular shape of the platelets, as observed in Figure 5.6. The emission polarization and emission pattern measurements have been then repeated with the second kind of nanoplatelets - the rectangular ones. The original idea is to understand if the shape of the nanoplatelet could have any influence on the polarization state of its emission.

Figure 5.15(c) shows a histogram of the obtained values of the degree of polarization δ of 18 individual rectangular nanoplatelets. The value of δ varies from 10% to 30%, higher than of the square nanoplatelets. This result suggests that the emission polarization is related mainly to the geometric aspect ratio of the nanoplatelet. The large variation of the histogram of the measured degree of polarization leads us to two hypotheses.

The first interpretation for this polarized emission is that the dipolar orientation of the two dimensional emitting dipole may be tilted (Θ 6= 0), which seems to be abnormal since

Intensity (norm.) # emitters

Rotating angle (°) Degree of polarization

0.6

FIGURE 5.15: Rectangular nanoplatelets: (a) Schematic of the objective-sample configuration.

(b) Measured polarimetric emission analysis with blue circles presenting normalized intensity as a function of the rotating angle \$ of the halfwave plate and a solid red line for the fitting of the experimental curve with Equation 5.5. (c) Histogram of degree of polarization δ measured for 18 nanoplatelets.

the nanoplatelet is supposed to lie on the substrate due to its morphological characteristics.

However, as the emitters are chemically synthesized, it may either result from defects in the crystalline structure or just because the platelet imperfectly horizontally lies on the substrate, as illustrated in Figure 5.16(a).

Another explanation of the polarized emission we propose, is that the two dimensional dipole can not be modelled by a sum of two degenerate orthogonal one dimensional dipoles (d1 = d2 =d), but by non-degenerate dipoles with d1 6=d2 (corresponds to d0

2

√1 +η and d0 2

√1−η in relative units), as described in 5.16(b). The possible values of the dipolar asymmetric factor η is from -1 to 1 as it is not necessary to know exactly which component dipole is oscillated more strongly.

5.4.2.2 Relevant hypotheses raised by emission pattern analysis

The present experimental configuration does not enable us to distinguish between these two hypotheses because their corresponding simulated emission patterns are quite similar. How-ever, the difference between these two ambiguous interpretations is clearly observed when we consider an other objective-sample configuration. Figure 5.16(c) illustrates the new interface configuration: The emitters are well spin-coated on the glass substrate and their emission is collected by an oil objective with the numerical aperture of 1.4 in contact with the side without emitters of the substrate. Since the refractive indices of glass and oil are very close to each other, it is considered as the nanoplatelets are at the air half-space of the air-glass interface.

The simulated Fourier plane images of a tilted two dimensional dipole with Θ = 30o and a non-degenerate dipole by a dipolar asymmetric factor η of 0.2 are described in Figure 5.16(d)

and (e) respectively.

FIGURE 5.16: The schematic representations of two interpretations for the nanoplatelet’s emitting dipoles (a,b) and their corresponding simulation of Fourier plane images (d,e) in the case of emitters directly positioned on glass substrate with an oil objective (N A- 1.4) in contact with the other side of the substrate as schematized in (c).

Both calculated images Figure 5.16(d) and (e) present a clear ring at the critical angle θc corresponding to the total internal reflection at the air-glass interface. However, there is a qualitative difference between these two images. In the pattern of a degenerate dipole oriented at Θ = 30o with respect to thezreference axis, the emission part inside this ring is asymmetric.

On the other hand, if the emitting dipole does not present the same energy along two different orthorgonal directions (a non-degenerate dipole), the emission part inside the ring has an axial symmetry while the ring itself no longer remains isotropic. Therefore, we perform the emission pattern measurements with the configuration described in Figure 5.16(c).

The measured Fourier plane image as presented in Figure 5.17 concides with the second hypothesis, indicating that the luminescence from rectangular nanoplatelets can be modelled as originating from a horizontal two dimensional dipole consisting of two non-degenerate one dimensional dipoles (d1 6=d2).

0 0.4 0.8

-0.8 -0.4

0 0.4

0.8 -0.4 -0.8

sin(θ)sin(ϕ)

sin(θ)cos(ϕ)

FIGURE 5.17: Emission pattern image measured from a rectangular nanoplatelet positioned on the glass substrate in contact with an oil objective as shematized in Figure 5.16(c).

5.4.2.3 Emission polarization analysis

Let us consider 2 linear dipoles d1 and d2 lying in the (x, y) plane, both of them have Θ1 = Θ2 = Θ = 90o; moreover, we assume that d1 has Φ01 = Φ +π/2 then for the case of d2, Φ02 = Φ +π, so that they are orthogonal.

As mentioned in the theoretical modelling, we could adjust the emitted photoluminescence signal as a function of the rotating polarization analyzing angle β as the followings:

P(β) =Pmin+ (PmaxPmin) cos20β) (5.6) with an one dimensional dipole

Pmin =A sin2Θ +B cos2Θ (5.7)

PmaxPmin =C sin2Θ (5.8)

where Pmin and Pmax stand for the minimum and maximum detected signals, and A, B, C could be calculated from the Fresnel reflective index (which is different in different cases of the interface configuration between the sample and the objective) and the numerical aperture of the objective.

In the case of an one dimensional dipole, Φ0 = Φ, the detected intensity is maximum when the axis of polarization β is aligned with the axis of the dipole (β = Φ). Since Θ = 90o, we could simplify P(β) = A+C cos2(Φ−β). Therefore, the total emitting power of the linear

dipole d1 and d2 respectively:

P1(β) = 1+|η| 2

A+C sin2(Φ−β) (5.9)

P2(β) = 1− |η | 2

A+C cos2(Φ−β) (5.10)

where η denoting the dipolar asymmetric factor corresponding to the difference between two component dipoles d1 and d2.

Finally, the total signal detected from a two dimensional dipole consisting of two non-degenerate one dimensional dipoles:

XP =P1(β) +P2(β)

= 1+ |η|

2 [A+C sin2(Φ−β)] + 1− |η|

2 [A+C cos2(Φ−β)]

=A+C

2 −C |η|

2 cos[2(Φ−β)]

(5.11)

As −1≤cos[2(Φ−β)]≤1 and 0≤|η| we have:

Pmin =A+ C

2 − C |η|

2 (5.12)

Pmax=A+ C

2 + C |η|

2 (5.13)

The degree of the linear polarization is defined as:

δ= PmaxPmin

Pmax+Pmin = C

2A+C |η| (5.14)

This linear theoretical relation between the degree of polarization of the emissionδand the dipolar asymmetric factor η of the emitting dipole is plotted in Figure 5.18(b). For example, in the case of a rectangular nanoplatelet placed on the glass substrate in contact with an oil objective as schematized in Figure 5.18(a), we obtain the degree of polarization of its emission δ= 0.15 from the polarimetric curve presented in Figure 5.18(c). Since C

2A+C ≈0.75 for the air-glass interface, it implies that the factor η = 0.2.

−1 0 1

FIGURE 5.18: (a) Schematic of the investigated objective-sample configuration. (b) Theoretical relation between the emission degree of polarization δ and the dipolar asymmetric factor η cal-culated for the air-glass interface. (c) Emission polarimetric curve measured from a rectangular nanoplatelet at air-glass interface.

5.4.2.4 Comparison between Emission polarization analysis and Emission pattern analysis

Futhermore, it is possible to determine the dipolar asymmetric factorη from the emission pattern measurement. Characterizing an individual rectangular nanoplatelet at the air-glass interface as illustrated in Figure 5.18(a), we plot the experimental emission pattern (circles) and then compare with the data simulated with different values ofη(solid lines) for a horizontal two dimensional dipole with in-plane orientation Φmax (green) and Φmax+ 90o (blue) in Figure 5.19 with Φmax is estimated from the polarimetric curve shown in Figure 5.18(c).

30°

FIGURE 5.19: Comparison of the measured emission pattern (cirles) from a rectangular nanoplatelet and the calculated emission pattern (solid lines) with a two dimensional dipole oriented at Θ = 0 and Φ = Φmax (extracted from the emission polarimetric curve of the same emitter) having the component strength ratio η along the direction of Φmax (green) and Φmax+ 90o(blue). The chosen configuration is the air-glass interface as illustrated in Figure 5.18(a).

The captured emission pattern is fitted the best whenη = 0.23. This agreement confirms that the hyphothesis of the rectangular nanoplatelets being a sum of two orthorgonal component

dipoles with different osillator strengths fits quantitatively with the experimental data. And when η < 0.15 or η > 0.3, the fitting obiviously gets worse. The factor η for this emitter is then determined to be between 0.15 and 0.3. Thus, this fitting analysis could estimate a factor η with a uncertainty of ±0.08. The accuracy is principally limited by the signal-to-noise ratio for the emission at small angles.

On the other hand, the factorηcan also be determined by emission polarization measure-ments with the uncertanity of:

= 2A+C

C (Θ) (5.15)

Since the uncertainty of the polarimetric measurements is (Θ) = 0.04, we have = 0.05.

0 0

η

from emission polarization

0.1 0.2 0.3

0.1 0.2 0.3

η from emission pattern

FIGURE 5.20: Comparison of the dipolar asymmetric factor η extracted from emission pat-tern measurement and from emission polarization measurement for 4 different rectangular nanoplatelets.

Figure 5.20 pictures the correspondance between the values of the dipolar asymmetric factor η extracted from emission polarization measurements (η is calculated from the experi-mental degree of polarization δ by Equation 5.22) and the values estimated by fitting analysis of the emission pattern for 4 different rectangular nanoplatelets. The linear function between two values confirms the correlation between two approaching ways in order to determine the dipolar orientation: emission polarimetric and emission pattern analysis.

Dans le document The DART-Europe E-theses Portal (Page 106-112)